4. Results and discussion
4.1 Powder monitoring
4.1.1 First cycle of the production process
56 Cycle 1
Virgin After PRS
Figure 4.1: Comparison of the flowability between (a) virgin sample (b) after one stage of PRS performed after the first cycle of EBM job.
As it is observable in figure 4.2-a, Ti-6Al-4V particles are surrounded by many satellites which is the typical feature of gas-atomized powders. At the first cycle it was observed that, in comparison with the virgin particles, characterized by the high quantity of satellites and smooth spherical forms without impurity, the powders after the first recycling undertook a little irregular form and some contaminations on the surface of the particles arisen from Fe.
Besides, sieving brings about a reduction of percentage of satellites because it removes agglomerated particles or partially sintered particles.
57 Figure 4.2: Morphological illustration of (a) virgin powder samples, (b) top and (c) bottom sintered powders and (d) after PRS performed after the first cycle of EBM job with magnifications of 500 x and 3000 x.
Figure 4.3 reports optical microscopy images of virgin, top and bottom sintered Ti-6Al-4V particles and powders after one stage of PRS performed after the first cycle of EBM job. The upper images are related to not-etched powders and reveal the presence of both irregular shapes (not perfectly spherical) and pore inside some particles. In particular, these internal pores derive from gas bubbles entrapped in molten metal during production processes of the same particles (gas atomization). If a bulk sample contains such gas pores, these derive from particles with gas pores inside. Instead, the bottom images in figure 4.3 represent the powder material etched with Kroll’s solution. The microstructure change of Ti-6Al-4V powders is related to the number of reused times. As shown in figure 4.3, the cross-section of the particles differs for each type of powders. For the virgin particles, the dominant phase is α or martensitic α’ and, after the first cycle of production, it would seem that the β phase appears in the structure of the particles; also, all cross-section images reveal that the particles have a thick lamellar structure.
58 Figure 4.3: Optical images of (a) virgin powder samples, (b) top, (c) bottom sintered powders and (d) after PRS during the first cycle of production in the states of un-etched (above) and etched samples (down) with magnifications of 100x and 200x, respectively.
Figure 4.4 illustrates the microstructure and oxidation conditions of virgin, top and bottom sintered powders and powders obtained after the recycling performed after the first cycle of EBM job. The microstructure before and after the first cycle of production changes; yet a basketweave and intergranular structures are observed. The thickness of lamellae in virgin powders (0.75 ± 0.32 μm) shows a slight increase compared with that obtained after the first recycling (0.86 ± 0.27 μm); instead, semi-sintered top and bottom powders reveal thicker lamellae than previous cases. After EBM process an opaque grey layer appears at the surface of the particles and in figure 4.4 is marked with a red arrow; this layer corresponds to oxide, which is formed after the building when the powders were still rather hot and the chamber is opened to extract the building.It should be remembered that oxygen enhances the fragility of the material and reduce flowability. The oxidized layer thickness is approximately the same both in top and bottom sintered powders.
59 Figure 4.4: SEM images of microstructure and oxidized layers in (a) virgin, (b) top and (c) bottom sintered Ti-6Al-4V powders and (d) in powders after one cycle of PRS performed after the first cycle of EBM job.
In figure 4.5 magnified images of a particle after the recycling performed after the first cycle of EBM job is shown. In figure 4.5-b and c, the reference line where the chemical composition analysis was carried out is indicated. It results that the α’ phase is rich in aluminium; indeed, Al belongs to the category of α-phase stabilizing elements, i.e. it moves the β-transus temperature up. Aluminium determined the nucleation and growth of those long and thick lamellae clearly observable in figure 4.5-b and c.
Figure 4.5: SEM images at different magnifications of a particle after the cycle of PRS performed after the first cycle of EBM job. The reference line for chemical composition analysis is also indicated.
a b c d
60 Figure 4.6 represents a magnified image of the microstructure of another powder obtained after the cycle of PRS. Also, the area where the chemical composition analysis was carried out is shown. As can be seen in this Figure, the white-coloured phase characterized by an irregular shape is rich in vanadium which is a β-phase stabilizing element. This finding clearly proofs that the powder is subjected to a thermal treatment that results in a partial phase transition.
Figure 4.6: SEM-EDS analysis of a particle after the first recycling step (after PRS).
Figure 4.7 represents the SEM images of some Ti-6Al-4V particles obtained after the first recycling step (after PRS). Thereafter, the cross-section of powder was analysed via SEM to investigate the surface oxidation of the particles. As it is clearly observed in figure 4.7-b, the oxide thickness is not uniform and the mean value of this oxide layer is 3.02 ± 1.39 μm. The chemical composition of the oxide and surface layer of the particle was measured with SEM-EDS analysis and taken from the line drawn in figure 4.7-c. The results are shown in figure 4.7-d. As expected, the oxygen amount increases towards the topmost region of the oxide layer. Instead, titanium and vanadium profiles exhibit negligible variations of composition along the depth direction. Interestingly, the aluminium quantity decreases towards the oxide layer and, in correspondence of it, the quantity of aluminium itself doesn’t vary anymore.
Figure 4.7: (a) SEM image of 6Al-4V particles after one stage of PRS. (b) SEM image of a Ti-6Al-4V particle and its oxide layer developed after the first cycle of PRS, with (c) indication of the reference line for the EDS chemical composition analysis. (d) Chemical composition trends of the elements oxygen, titanium, aluminium and vanadium along the radial direction of the same particle.
62 The SEM-EDS examination of Ti-6Al-4V powders produced by gas atomization process and recovered by the PRS system doesn’t reveal just the presence of titanium, aluminium and vanadium. Indeed, in correspondence of irregularities, visible on the surface of some particles, relevant presence of iron was detected (figure 4.8). This element represents clearly a contaminant and normally its amount is limited at a maximum of 0.3%. The effect of iron in titanium alloys is to stabilize β phase with the appearance of a eutectoid reaction in proximity of thermodynamic equilibrium conditions. It moves the β → α transformation temperature down and may change the probability to find a specific microstructure in determined conditions of cooling. A secondary effect of iron on titanium alloys is to enhance the coagulation rate of intermetallic compound, that decreases the strength and increases the ductility of the material . The probable sources of iron contamination could be from the
“metallization” particles that probably fall down inside the building envelope and contaminated the powders. Contamination of iron could represent a serious problem in case of application of materials in biomedical fields because this element is not fully biocompatible.
Figure 4.8: SEM images of Ti-6Al-4V particles after the first PRS cycle, containing some iron contaminants on their surface. The way EDS chemical composition analysis has been performed and their results are also reported.
Figure 4.9 reports in a histogram the EDS results relative to weight concentrations of titanium, aluminium and vanadium obtained in virgin, top and bottom sintered Ti-6Al-4V powders and obtained in the same material after one cycle of PRS. The weight concentration of oxygen has been analysed, but just in top and bottom sintered powders and powders after one cycle of PRS. The pick-up of oxygen gradually increases by the end of the recycling steps.
63 Figure 4.9: Chemical composition changes of Ti-6Al-4V powders during different stages of process (virgin state, sinter top, sinter bottom and after the first cycle of PRS).
Figure 4.10 reports the results of XRD analysis, both in diffractogram and in chart form, of the virgin and sintered powders of Ti-6Al-4V and the same alloy after one cycle of PRS. All peaks are related to the α phase (HCP); the most important one corresponds to an angle 2θ ≈ 40° and it has been used to calculate the average crystal size with Scherrer’s formula:
τ= β cos θK λ (4.1)
where τ corresponds to the average size of grains, K is a shape factor near unity (the most used value is 0.9), λ is the x-ray wavelength incident on the sample, β is the full width at half maximum (FWHM), θ is Bragg’s angle. The peak after the EBM process has become taller and narrower than the one related to virgin material. The results demonstrate a crystal coarsening after EBM process. A slight decrease of crystallinity is verified in powders subjected to one cycle of PRS with respect to those taken just after EBM process.
Figure 4.10: (a) XRD resulting from virgin, sintered and after PRS Ti-6Al-4V powders and the consequent average crystal size plot (b).